received: 18 December 2015 accepted: 20 May 2016 Published: 07 June 2016
Design of Hydrogen Storage Alloys/Nanoporous Metals Hybrid Electrodes for Nickel-Metal Hydride Batteries M. M. Li, C. C. Yang, C. C. Wang, Z. Wen, Y. F. Zhu, M. Zhao, J. C. Li, W. T. Zheng, J. S. Lian & Q. Jiang Nickel metal hydride (Ni-MH) batteries have demonstrated key technology advantages for applications in new-energy vehicles, which play an important role in reducing greenhouse gas emissions and the world’s dependence on fossil fuels. However, the poor high-rate dischargeability of the negative electrode materials—hydrogen storage alloys (HSAs) limits applications of Ni-MH batteries in highpower fields due to large polarization. Here we design a hybrid electrode by integrating HSAs with a current collector of three-dimensional bicontinuous nanoporous Ni. The electrode shows enhanced high-rate dischargeability with the capacity retention rate reaching 44.6% at a discharge current density of 3000 mA g−1, which is 2.4 times that of bare HSAs (18.8%). Such a unique hybrid architecture not only enhances charge transfer between nanoporous Ni and HSAs, but also facilitates rapid diffusion of hydrogen atoms in HSAs. The developed HSAs/nanoporous metals hybrid structures exhibit great potential to be candidates as electrodes in high-performance Ni-MH batteries towards applications in new-energy vehicles. Recently, with increasing pressures of environmental problems and energy crisis, more and more sights have turned to new-energy vehicles1–3. A series of advanced battery technologies have been emerged for applications in this field, nickel metal hydride (Ni-MH) batteries, Li-ion batteries, proton exchange membrane fuel cells etc4–6. Ni-MH batteries were first commercialized and they were facing great challenges from Li-ion batteries over the past few years. Nonetheless, Ni-MH batteries still hold an important position in the market, especially in hybrid electric vehicles, due to their superior safety even under abuse conditions, temperature adaptability and environmental friendliness7–9. Moreover, Ni-MH batteries have also been widely used in the fields of power tools and modern military devices10,11. A moderate energy density is sufficient while a high power density is critical for these applications. To meet the marketing requirements for high-power Ni-MH batteries, one has to enhance the high rate dischargeability (HRD) properties of their negative electrode materials—hydrogen storage alloys (HSAs), which determine the power density of Ni-MH batteries. It should be noted that although supercapacitors have high power density, the low energy density at present makes it only a complement to batteries in energy storage devices12. In the last two decades, various approaches have been proposed to improve the electrochemical properties of HSAs, such as composition optimization13, surface modification14,15, preparation techniques modification16, processing methods optimization17 etc. The surface modification has been demonstrated as an efficient approach to enhance the HRD performance of HSAs. The traditional surface modification methods, such as acid, alkaline and fluorination treatments, could dissolve rare earth oxides or hydroxides on the surface of alloy particles. The active elements (for example, Al and Mn) are also etched to form a Ni-rich porosity layer, which is useful for accelerating the electrochemical reaction rate14,15. Several groups have reported the improvements in HRD of alloy electrodes by microencapsulating alloy particles with various coating layers, Ni, Cu, Co, Ni-P, and so on, via the electroless technic18–25. It was reported that the plated Cu and Ni could act as microcurrent collectors to increase the charge transfer rate on electrode surfaces and as barriers to protect alloy particles from oxidation18,19. The Ni-Co deposits Key Laboratory of Automobile Materials (Jilin University), Ministry of Education, and School of Materials Science and Engineering, Jilin University, Changchun 130022, China. Correspondence and requests for materials should be addressed to C.C.Y. (email: [email protected]
) or Q.J. (email: [email protected]
Scientific Reports | 6:27601 | DOI: 10.1038/srep27601
Figure 1. A schematic illustration of the preparation of HSAs/NPNi composite by using a top-down method. (a) The preparation process of the HSAs/NPNi composite. (b) The photograph of an electrode pellet for electrochemical measurements. could work as catalysts to improve the electric catalytic activity of HSAs23. Moreover, the electroless plating of Ni-P nanoparticles on alloy surfaces has been demonstrated to be beneficial for decreases of contact resistance and charge transfer resistance of the electrode25. Mechanical milling has also been introduced to improve the HRD of hydride electrodes26. Moreover, carbon nanotube, graphite, and nickel nanoparticles were added into HSAs to form hybrid electrodes27–29. Note that the hybrid electrode is prepared by compositing two or more different materials (in general, at least one constituent is at the nanometer scale) into a single electrode and it shows new properties not necessarily found in the individual parent components. The additives show remarkable positive effects on accelerating the absorption and desorption of hydrogen atoms, increasing the electrochemical reaction rate27. All these modification methods have been proved to be effective in improving the HRD performance of hydride electrodes, but the improvements are limited26,27. Moreover, they bring some disadvantages, for example, the deformation and amorphization of HSAs26. The current commercial Ni-MH battery in hybrid electric vehicles only deliver the specific power of 150–400 W/kg, which cannot satisfy the increasing marketing requirements8,30. The Department of Energy of US has set a target of over 650 W/kg31. Thus, it is urgent to explore the intrinsic factor that dominates the HRD properties of HSAs, and to develop novel materials to achieve the above target. Conventionally, the metal hydride electrodes for electrochemical measurements are prepared by cold pressing the mixture of HSA powders and copper or nickel powders (as current collector and binder)27. In this regard, a large contact resistance (RC) between current collector and active materials, or within active materials, a large charge transfer resistance (RCT) and a large mass transport resistance (RMT) exist during the electrochemical reaction of electrodes32. The large internal resistances lead to large polarization and poor electrochemical properties. Recently, nanoporous metals have demonstrated potential technological advantages to reduce the above internal resistances due to their unique porous structures with large surface/volume ratio32,33, which have been successfully used in supercapacitors34, electrochemical catalysts35,36, Li-ion batteries37 and other energy storage devices38. The HRD performance of a metallic hydride electrode is mainly determined by two steps: the electrochemical reaction on the surface of alloy electrode (charge transfer process) and the diffusion of absorbed hydrogen into the alloy bulk (hydrogen diffusion process)39. These two steps are closely related to exchange current density (I0), electrochemical impedance and hydrogen diffusion coefficient (DH). A higher I0 value corresponds to a better kinetics of absorbed and desorbed hydrogen, a smaller polarization resistance and a faster charge transfer process40. A larger DH allows for a faster transportation of absorbed hydrogen and a faster hydrogen diffusion process. Nanoporous metals have unique porous structures with large surface/volume ratio. Hence, they could be used to (i) increase the electrochemical active area and thus to improve electrochemical reaction kinetics; and (ii) decrease the internal resistance and polarization and thus to enhance the conductivity of a metallic hydride electrode. Integrating nanoporous metals with HSAs powders is expected to enhance the HRD performance of HSAs. This approach has not been reported before and it opens a door to applications of nanoporous metals in Ni-MH batteries. The major aim of this work is to develop a new type of hybrid electrode (HSAs/NPNi) by incorporating HSAs powders with a current collector of three-dimensional bicontinuous nanoporous Ni for applications in Ni-MH batteries. Such a composite shows excellent HRD performance where its discharge capacity is 2.4 times that of the bare HSAs at a discharge current density of 3000 mA g−1. It is found that the NPNi introduced into the composite decreases RC and RCT, and accelerates the diffusion rate of hydrogen atoms in HSAs. The findings in this work provide a new strategy to improve the HRD performance of Ni-MH batteries, which can also be utilized to design other electrode materials.
Results and Discussions
The HSAs/NPNi hybrid electrode pellets were fabricated with a facile procedure, which involves hydrothermal synthesis of Ni(OH)2, integration of Ni(OH)2 with the master alloy (LaCe)0.9Y0.1Ni3.7Co0.75(MnAl)0.65, thermal reduction of Ni(OH)2 by annealing treatment of the composites under an Ar/H2 atmosphere, and cold pressing the mixture of as-prepared composites and carbonyl nickel powders (Fig. 1a,b). Figure 2a shows X-ray diffraction (XRD) patterns of the master alloy and the composite. It is evident that the master alloy retains a typical Scientific Reports | 6:27601 | DOI: 10.1038/srep27601
Figure 2. Morphological and microstructure characterizations of the master alloy and HSAs/NPNi composite. (a) XRD patterns of the master alloy and HSAs/NPNi composite. (b–d) are top-view SEM images of surfaces of the master alloy, composite and NPNi, respectively. (e,f) (including the inset) are TEM and HRTEM images of NPNi.
CaCu5-type crystalline structure with a space group of P6/mmm41. The XRD pattern of the composite shows characteristic peaks of Ni besides the LaNi5 phase. Moreover, it is found that the peaks of Ni phase are broadened, which is attributed to the formation of nanoscale polycrystals [NPNi as demonstrated by scanning electron
Scientific Reports | 6:27601 | DOI: 10.1038/srep27601
Figure 3. Discharge capacities and HRD properties. (a) The discharge capacity curves of the HSAs/NPNi hybrid electrode and master alloy electrode at room temperature. (b) The HRD properties of the HSAs/ NPNi hybrid electrode and master alloy electrode at different discharge current densities measured at room temperature. (c) Comparisons of HRD properties of the HSAs/NPNi composite and reported experimental data of AB5-type HSAs from other advanced surface modification methods, including carbon nanotube (CNT) doping (CNT-1 wt% and CNT-0.05 wt%) for MmNi3.6Co0.7Al0.3Mn0.427, fluoridation treatment (F-treated), fluoridation and the following treatment with KBH4 (F-treated & KBH4) for MlNi3.8Co0.75Mn0.4Al0.215, combination of fluoridation treatment and elelctroless plating with Ni-P coating (F-treated & Ni-P) for LaNi4Al25, hot alkaline treatment at 100 °C (KOH), electroless with nickel coating (Ni coating), and combination of alkaline treatment and electroless with Ni coating (KOH & Ni) for MmX4.3(Al0.3Mn0.4)0.5 (X = Co, Mo, Mn, Al, Cu)14. (d) A comparison of ratios of HRD performance after treatment to that of untreated HSAs between NPNi incorporation and CNT doping.
microscope (SEM) and transmission electron microscope (TEM) images below] during the annealing treatment42. The weight percent of NPNi in the composite is 36.87% as measured by an inductively coupled plasma (ICP) analyzer. Note that the weight percent (y) of original Ni (of master alloy) in the composite is determined by comparing with the contents of La, Ce, Y, Co, Mn and Al. For example, the Co content in the composite was measured by ICP as x (=6.48%) and we have y = 5.01x = 32.47% (the weight percent ratio of Ni to Co in the master alloy is 5.01). The total Ni content in the composite is z = 69.34% as measured by ICP. Then, the weight percent of NPNi in the composite (z-y = 36.87%) is obtained. The morphologies of as-fabricated samples are characterized by a field-emission SEM (FESEM) and a TEM. Figure 2b shows an SEM image of the master alloy, where clean surfaces could be observed. On the contrary, as shown in Fig. 2c, the master alloy particle is surrounded by NPNi in the composite, exhibiting rough surfaces. The NPNi with pore size of ~200 nm and ligament size of ~120 nm is formed during the reduction of Ni(OH)2 (Fig. 2d). Figure 2e shows a TEM image of NPNi at a low magnification. Combining Fig. 2d,e, we can find that (1) NPNi has a three-dimensional bicontinuous nanostructure; and (2) NPNi ligaments show a hyperboloid-like shape, where a positive curvature forms columnar ligaments while a negative curvature accommodates nanopores43,44. Note that the nanopores and ligaments in nanoporous metals or intermetallics are topologically and morphologically equivalent, i.e., they are inverses in a three-dimensional space, resulting in a near-zero surface curvature on average. Such a structure is typically called bicontinuous structure due to its continuous nanopore channels and ligaments. Figure 2f presents a high-resolution TEM (HRTEM) image of NPNi, in which the interplanar spacings of 0.203, 0.233 and 0.176 nm correspond to (111), (010) and (200) (inset of Fig. 2f) planes of Ni, respectively. Figure 3a shows the discharge capacity curves of the master alloy electrode and HSAs/NPNi hybrid electrode at a discharge current density of 60 mA g−1 (0.2C). The measured maximum discharge capacity Cmax values are 257.51 mAh g−1 and 222.14 mAh g−1 for the master alloy and composite electrodes, respectively, which are listed
Scientific Reports | 6:27601 | DOI: 10.1038/srep27601
Cmax (mAh g−1) HRD3000 (%) RC (mΩ) RCT (mΩ) I0 (mA g−1) IL (mA g−1) DH (×10−10 cm2 s−1)
Table 1. Electrochemical properties of the HSAs/NPNi hybrid electrode and master alloy electrode.
in Table 1. It is known that the reactions of a metal hydride electrode during charging are typically described by (1) the Volmer reaction: H2O + e− → Hads + OH−; (2) the transition of hydrogen atoms between adsorbed state and absorbed state on the surface of alloy particles: Hads → Habs; and (3) the following phase transformation process: MHα → MHβ31. Note that the order of the above reactions is on the contrary during the discharging process. Apart from these reactions, there is also a hydrogen evolution reaction (HER) by the Volmer-Tafel reaction route (H2O + e− → Hads + OH− and the following 2Hads → H2) or by the Volmer-Heyrovsky reaction route (H2O + e− → Hads + OH− and the following Hads + H2O + e− → H2 + OH−) during charging45. It has been demonstrated that NPNi could act as a catalyst to accelerate the HER reaction46. As a result, during charging, Hads as a product of the Volmer reaction fast recombined to generate H2 in the composite, which results in (1) a decrease of the number of Hads to diffuse into the HSAs to create hydrides; and (2) a reduction of the utilization rate of active materials. In this case, during discharging, the reactant Hads (Hads + OH− → H2O + e−) becomes less, leading to a smaller Cmax value of the composite compared with the master alloy. Figure 3b shows the HRD property of the both electrodes. The corresponding electrochemical data are listed in Table 1. The capacity retention rates of the composite electrode are 102.6, 96.6, 92.1, 83.2, 75.2, 58.4 and 44.6% at the discharge current densities of 300, 600, 900, 1200, 1500, 2400 and 3000 mA g−1, respectively, showing better HRD performance than that of the master alloy electrode (the corresponding capacity retention rates are 94.7, 84.4, 73.9, 66.6, 58.5, 29.5 and 18.8%). At the discharge current density of 3000 mA g−1 (10C), the capacity retention rate of the composite is 2.4 times that of the master alloy. As noted above, the Cmax value of the composite at 0.2C is lower than that of the master alloy. But the discharge capacity of the former at 10C (98.99 mAh g−1) is twice that of the latter (48.39 mAh g−1). Moreover, it should be noted that the discharge capacity (228.02 mAh g−1) of the composite at 1C (300 mA g−1) is a little larger than the capacity (222.14 mAh g−1) at 0.2C (60 mA g−1). This may result from stronger hydrogen evolution during charging at higher discharge current density (1C) than that at lower current density (0.2C)19. In the discharging process, the dissolved hydrogen is ionized in the electrolyte and an additional charge contributes to the overall value, causing larger discharge capacity of the composite electrode at 1C than that at 0.2C19. Note that their difference is very small (5.88 mAh g−1), which indicates that (1) most of hydrogen has escaped from the electrolyte in the open system of a half-cell test; and (2) contributions of the ionization of hydrogen to discharge capacities of the master alloy and composite electrodes are limited although the both electrodes show different catalytic activity for the HER reaction. For a comparison, we have also fabricated the electrode using bare HSAs without annealing under an Ar/H2 atmosphere and tested its electrochemical properties. It shows larger discharge capacity (302.62 mAh g−1) while poorer HRD performance (the capacity retention rate at 10C is 13.5%) compared with the master alloy and composite electrodes47,48. Figure 3c compares the HRD performance of HSAs/NPNi composite and reported experimental data of AB5-type HSAs from other advanced treatment methods, hot alkaline etching at 100 °C (KOH), electroless plating with Ni coating, and their combination for MmX4.3(Al0.3Mn0.4)0.5 (X = Co, Mo, Mn, Al, Cu)14, carbon nanotube (CNT) doping for MmNi3.6Co0.7Al0.3Mn0.427, fluoridation treatment, fluoridation and the following treatment with KBH4 for MlNi3.8Co0.75Mn0.4Al0.215, combination of fluoridation treatment and elelctroless plating with Ni-P coating for LaNi4Al25 etc. It can be seen that the HSAs/NPNi composite shows similar HRD performance as CNT-doped HSAs and notable superiority than other surface modification methods. Moreover, the incorporation of NPNi has better enhancement effect on the HRD properties of HSAs than CNT doping, especially when discharge current densities are larger than 1500 mA g−1 as shown in Fig. 3d, which plots the ratios of their HRD property after treatment to that of untreated HSAs. On one hand, this is owing to the excellent contact between NPNi and HSAs in our composite, which is beneficial for decreases of the internal resistance and polarization. On the other hand, the NPNi provides numerous active sites for the adsorption of OH− and also accelerates transfer rates of the electron and ion due to its unique three-dimensional bicontinuous structure, both of which are beneficial for the enhanced electrochemical reaction kinetics. Figure 4 further compares the discharge capacity curves of master alloy electrode and HSAs/NPNi hybrid electrode at different discharge current densities of 1C, 5C, 8C and 10C. It is evident that the discharge capacities of the both electrodes decrease with increasing discharge rate. Although the composite electrode has lower discharge capacity than that of the master alloy electrode at 1C, it is quite the opposite at larger discharge rates (5C, 8C and 10C), which indicates the enhanced HRD properties of the composite electrode. Moreover, the discharge potential plateau of the composite electrode is higher than that of the master alloy electrode at each discharge rate, which demonstrates higher surface activity and smaller polarization of the former49. To explore the nature which underpins the superior HRD performance of the HSAs/NPNi hybrid electrode compared with bare HSAs electrode, we measured their linear polarization curves, electrochemical impendence spectra (EIS), anodic polarization curves and potential steps. Figure 5a presents linear polarization curves of the both electrodes. When the overpotential η changes within a small range (